Download presentation

Presentation is loading. Please wait.

Published byCaroline Biddulph Modified over 2 years ago

1
Lecture 2. Granular metals Plan of the Lecture 1)Basic energy scales 2)Basic experimental data 3)Metallic behaviour: logarithmic R(T) 4)Insulating behaviour: co-tunneling and ES law 5)Co-tunneling and conductance of diffusive wire Review: I.Beloborodov et al, Rev. Mod.Phys.79, 469 (2007)

2
g ≈ const Examples: Phys Rev B 1987 Phys Rev B 1981 Grain radius a >> λ F

3
Basic energy scales Grain radius a is large on atomic scale: k F a >> 1 Level spacing inside grain δ = 1/( 4a 3 ) Coulomb energy E c = e 2 /a Intra-grain Thouless energy E th = ћD 0 /4a 2 δ << E th << E c Example: Al grains with a=20 nm δ = 0.02 K E th = 50 K E c = 1000 K g 0 = E th / δ = 2500 Typical temperature range 4 K < T < 300 K Γ ~ 1K for g T = 50

4
Intergrain coupling Low transmission, but large number of transmission modes σ T = (4π e 2 / ћ) 2 g T = σ T h/e 2 - dimensionless inter-grain conductance A) Granular metal g T ≥ 1 B) Granular insulator g T ≤ 1 Narrow coherent band Γ = g T δ << E th Effective diffusion constant D eff = Γ a 2 /ћ << D 0 Γ~ 1K for g T = 50 Nearest-neighbors coupling only !

5
Experimental data: granular metals Phys Rev B 36 1964 (1987) Phys Rev Lett.78, 4277 (1997) R(T) = R 0 ln(T 0 /T) Coefficient in front of the Log is too large for interference corrections (Lecture 1)

6
Experimental data: granular insulators Phys Rev B 23 6172 (1981) Variable-range hopping in presense of Coulomb gap Efros-Shklovsky The origin of VRH ???

7
3) Metallic behaviour: theory of logarithmic R(T) dependence Granular structure leads to a new (compared to usual metals) energy window Γ << T << E C where - Coulomb energy is very important - Coherent nature of transport is irrelevant Useful formulation of the theory is in terms of phase variables φ i (t) = (e/ћ) ∫ t V i (t’)dt’ conjugated to grain charges Q i The reason: at g T >> 1 phases are weakly fluctuating

8
Ambegaokar-Eckern-Schön functional Phys Rev B 30, 6419 (1984) (¼) Action functional in imaginary (Matsubara) time

9
Perturbation theory Quadratic approximation for the action: G -1 = (ω n 2 /2e 2 ) C(q) + (1/π) g T |ω n | β(q) β(q) = Σ a ( 1- cos qa )ω n = 2 π n T ~ (1/ g T ) Σ n (1-cos ω n τ)/[ |ω n | + ω n 2 /E C g T ] High-energy cutoff E C g T = 1/(RC) Low-energy cutoff 1/ τ ~ (1/ g T ) ln (E C g T τ)

10
Intergain conductivity

11
1 st logarithmic correction: g T (T) = g T – (4/z) ln (g T E C /T) here z is the lattice coordination number The origin of this correction: discreteness of charge transfer. Formally, it is represented as non-linearity of the AES action in phase representation. Phase (voltage) fluctuations across each tunnel junction destroy coherence of electron states in neighboring grains, and suppress inter-grain conductivity. Contrary to usual logarithmic corrections in 2D metals, this effect does not depend on dimensionality

12
Renormalization group (¼) Split phase variables into slow and fast parts

13
Renormalization group -2 - 4/z Valid as long as g ≥ 1

14
Conclusion from RG analysis: g T (T) = g T – (4/z) ln (g T E C /T) The solution is valid down to T* ≈ g T E C exp[-(z/4)g T ] where g T (T*) ~ 1 (1) R(T) = R 0 ln(T 0 /T) Solution (1) does not coinside with experimental result

15
What is the reason for disagreement ? 1. R(T) approaching R K =h/e 2 Ratio thickness/2a ~ 5 g T (300K) ~ 2g T (10K) ~ 0.5 Condition g T >> 1 is not fulfilled 2. Distribution of local g ij is broad due to fluctuations of

16
RG for disordered granular array M.Feigelman, A.Ioselevich, M.Skvortsov, Phys.Rev.Lett. 93, 136403 (2004) Random initial values of tunneling conductances g ij Generalized RG equation instead of is the actual resistance between grains i and j

17
RG for disordered array: solution 1) Relative width of the P(g) grows fastly under RG : perturbation theory

18
RG for disordered array: solution-2 2) Strong disorder: effective-medium approximation Explicit solution for symmetric distributions of ~

19
RG for disordered array: solution-3 “Universal temperature dependence of the conductivity of a strongly disordered granular metal” A. R. Akhmerov, A. S. Ioselevich JETP Lett. 83(5), 211-216 (2006); cond-mat/0602088cond-mat/0602088 Universal solution: Conclusion: strong disorder in h ij might be a reason for R(T) = R 0 ln(T 0 /T)

20
4) Insulating behaviour: co-tunneling and Efros-Shklovsky law Usual hopping insulator (doped semiconductor): Mott law t ij ~ exp(- r ij /a)a is the localization length of Hydrogen-like orbital P ij ~ exp(- 2 r ij /a) exp(- ε ij /T) ε ij is the energy difference between states i and j ε ij ~ ( r ij ) -d Optimize over r ij : min R (2R/a + 1/R d T) P opt ~ exp[-(T M /T) a ] a = 1/(d+1) Doped semiconductor with a Coulomb gap: ES law (ε) ~ ε d-1 ε(R) ~ 1/R Now R opt is found from min R (2R/a + const/RT) P opt ~ exp [-(T 0 /T) 1/2 ] T 0 = C e 2 /κa

21
Co-tunneling: correlated tunnling G orto ~ min(g L,g R ) exp(-E C /T) Consider now 2-nd order amplitude with charged grain in a virtual state (Averin & Nazarov PRL 65, 2446, 1990) Review:cond-mat/0501007 Level widths:

22
Co-tunneling: inelastic and elastic Inelastic: Number of terms ~ T/δE Elastic:

23
L is the number of “inelastic” grains N is the total grain number in the path General expression can be analyzed for local Coulomb only (screening by gate)

24
- limiting cases is the average conductance between neigbouring grains Usual optimization over N and ε leads to with and

25
Variable-range co-tunneling: estimates Example: Al grains with a=20 nm δ = 0.02 K E th = 50 K E c = 1000 K With g ~ 0.3 one finds L ≈ 10 Thus T ES ≈ 10 4 K and T c ≈ 0.5 K Conclusions: inelastic co-tunneling dominates, magneto-resistance is very weak

26
5) Co-tunneling and conductance of weakly coupled quasi-1D wire M.V.Feigel'man and A.S.Ioselevich, JETP Lett. 88, 767-771 (2008); arXiv:0809.1325arXiv:0809.1325 Experimental results: Usual view: “Luttinger Liquid” However, such a scaling is observed for multi-channel diffusive conductors Our explanation: inelastic co-tunneling + Coulomb anomaly

27
Total classical resistance We consider relatively high temperatures, i.e. no Anderson localization: max (T,eV) ------------- E C (L) () where Exponentially suppressed in L/ξ - in spite of the absence of localization

28
Coulomb zero-bias anomaly A.Finkelstein ZhETF 1984 Yu.Nazarov ZhETF 1989 L.Levitov & A.Shytov cond-mat/9607136 is the Action of charge spreading process U q = 2πe 2 /q J(q,ω) Potential energySource term: Usual result in quasi-1D:

29
Coulomb anomaly + inelastic co-tunneling J(q,ω)

Similar presentations

Presentation is loading. Please wait....

OK

Dynamics of Anderson localization

Dynamics of Anderson localization

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on foreign exchange market in india Ppt on complex numbers class 11th Free ppt on mobile number portability pdf Ppt on decimals for class 4 Editing ppt online Ppt on bionics medical Ppt on classical economics wikipedia Urinary tract anatomy and physiology ppt on cells Ppt on hard work is the key to success Ppt on cash reserve ratio